#------------------------------------------------------------------------------
#$Date: 2015-01-27 21:58:39 +0200 (Tue, 27 Jan 2015) $
#$Revision: 130149 $
#$URL: svn://www.crystallography.net/cod/cif/1/00/04/1000497.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1000497
loop_
_publ_author_name
'Renaudin, J'
'Ferey, G'
'de Kozak, A'
'Samouel, M'
_publ_section_title              'Structure cristalline de Ba2 Zn7 F18'
_journal_coden_ASTM              RVCMA8
_journal_name_full               'Revue de Chimie Minerale'
_journal_page_first              497
_journal_page_last               507
_journal_volume                  23
_journal_year                    1986
_chemical_formula_structural     'Ba2 Zn7 F18'
_chemical_formula_sum            'Ba2 F18 Zn7'
_chemical_name_systematic        'Barium zinc fluoride (2/7/18)'
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                94.24(2)
_cell_angle_beta                 92.82(2)
_cell_angle_gamma                116.39(2)
_cell_formula_units_Z            1
_cell_length_a                   7.032(2)
_cell_length_b                   7.292(2)
_cell_length_c                   7.505(2)
_cell_volume                     342.3
_exptl_crystal_density_meas      5.17
_refine_ls_R_factor_all          0.066
_cod_database_code               1000497
loop_
_symmetry_equiv_pos_as_xyz
x,y,z
-x,-y,-z
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_symmetry_multiplicity
_atom_site_Wyckoff_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_attached_hydrogens
_atom_site_calc_flag
Ba1 Ba2+ 2 i 0.3160(1) 0.6877(1) 0.6320(1) 1. 0 d
Zn1 Zn2+ 1 b 0. 0. 0.5 1. 0 d
Zn2 Zn2+ 2 i 0.1916(1) 0.8715(1) 0.1791(1) 1. 0 d
Zn3 Zn2+ 2 i 0.8217(1) 0.6198(1) 0.8062(1) 1. 0 d
Zn4 Zn2+ 2 i 0.6104(1) 0.7331(1) 0.1240(1) 1. 0 d
F1 F1- 2 i 0.4785(7) 0.5614(7) 0.3224(6) 1. 0 d
F2 F1- 2 i 0.1085(7) 0.7713(7) 0.9241(6) 1. 0 d
F3 F1- 2 i 0.7162(7) 0.9888(7) 0.5565(6) 1. 0 d
F4 F1- 2 i 0.9187(7) 0.7177(7) 0.5721(6) 1. 0 d
F5 F1- 2 i 0.9071(7) 0.8728(7) 0.2390(6) 1. 0 d
F6 F1- 2 i 0.7036(7) 0.8238(7) 0.8800(6) 1. 0 d
F7 F1- 2 i 0.1027(7) 0.6046(7) 0.2848(6) 1. 0 d
F8 F1- 2 i 0.4972(7) 0.9275(7) 0.1839(6) 1. 0 d
F9 F1- 2 i 0.6788(7) 0.4861(7) 0.0258(6) 1. 0 d
loop_
_atom_type_symbol
_atom_type_oxidation_number
Ba2+ 2.000
Zn2+ 2.000
F1- -1.000
